| ||Format||Pages||Price|| |
|11||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||11||$50.00||  ADD TO CART|
Significance and Use
NTA is one of the very few techniques that are able to deal with the measurement of particle size distribution in the nano-size region. This Guide describes the NTA technique for direct visualization and measurement of Brownian motion, generally applicable in the particle size range from several nanometers until the onset of sedimentation in the sample. The NTA technique is usually applied to dilute suspensions of solid material in a liquid carrier. It is a first principles method (that is, calibration in the standard understanding of this word, is not involved). The measurement is hydrodynamically based and therefore provides size information in the suspending medium (typically water). Thus the hydrodynamic diameter will almost certainly differ from size diameters determined by other techniques and users of the NTA technique need to be aware of the distinction of the various descriptors of particle diameter before making comparisons between techniques (see 8.7). Notwithstanding the preceding sentence, the technique is routinely applied in industry and academia as both a research and development tool and as a QC method for the characterization of submicron systems.
1.1 This guide deals with the measurement of particle size distribution of suspended particles, from ~10 nm to the onset of sedimentation, sample dependent, using the nanoparticle tracking analysis (NTA) technique. It does not provide a complete measurement methodology for any specific nanomaterial, but provides a general overview and guide as to the methodology that should be followed for good practice, along with potential pitfalls.
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C322 Practice for Sampling Ceramic Whiteware Clays
E456 Terminology Relating to Quality and Statistics
E1617 Practice for Reporting Particle Size Characterization Data
E2490 Guide for Measurement of Particle Size Distribution of Nanomaterials in Suspension by Photon Correlation Spectroscopy (PCS)
ISO StandardsISO 22412 Particle Size AnalysisDynamic Light Scattering (DLS)
ICS Number Code 07.030 (Physics. Chemistry)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E2834-12, Standard Guide for Measurement of Particle Size Distribution of Nanomaterials in Suspension by Nanoparticle Tracking Analysis (NTA), ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top